Effect of bonding duration and substrate temperature in copper ball bonding
on aluminium pads: A TEM study of interfacial evolution
H. Xu a, *, C. Liu a , V.V. Silberschmidt a , Z. Chen b , J. Wei c , M. Sivakumar d
a Wolfson School of Mechanical and Manufacturing Engineering, Loughborough University, Loughborough, LE11 3TU, UK
b School of Materials Science and Engineering, Nanyang Technological University, Nanyang Avenue, Singapore 639798, Singapore
c Singapore Institute of Manufacturing Technology, 71 Nanyang Drive, Singapore 638075, Singapore
d ASM Technology Singapore, 2 Yishun Avenue 7, Singapore 768924, Singapore
Received 31 January 2010
Received in revised form 24 March 2010
Accepted 24 March 2010
Available online 15 May 2010
There is growing interest in Cu wire bonding for fine pitch
application due to cost saving and better mechanical and electrical
properties. In this process, a thin copper wire is bonded to an aluminium
metallization pad using a combination of ultrasonic energy,
pressure ( 150 MPa) and heat (150–220 °C). It is a complex
process, and the physics has not been fully understood. However,
many efforts have been made to study and explain the process
[1–16]. In general, three experimental approaches have been used
to investigate the mechanisms of the bond formation. The first one
concentrates on experimentally in situ measurements of interfacial
temperature during bonding [1–3]. The second one considers an
explanation of characteristics of the observed footprints on the
bond pads or the bottom of bonds [4–9]. The third one is based
on the cross-sectional characterization of the interfacial microstructure
in wire bonds [10–12]. The main proposed theories include
melting , fretting  and micro-slip [15,16]. Melting
was postulated that ultrasonic vibration caused rubbing between
a wire and a pad, resulting in significant increase of the interfacial
temperature, so melting took place in local areas, leading to bonding
. However, there are a quantity of experimental evidences
to show that although there is a temperature rise, it does not
approach the melting point of the materials. For example, the
highest measured interfacial temperature during bonding by far
is 320 °C , and it is far below the melting point of bonding
* Corresponding author. Tel.: +44 (0) 1509 227684.
E-mail addresses: H.Xu3@lboro.ac.uk, firstname.lastname@example.org (H. Xu).
0026-2714/$ - see front matter Ó 2010 Elsevier Ltd. All rights reserved.
Microelectronics Reliability 51 (2011) 113–118
Contents lists available at ScienceDirect
journal homepage: www.elsevier.com/locate/microrel
The effect of bonding duration and substrate temperature on the nano-scale interfacial structure for
bonding strength were investigated using high resolution transmission electron microscopy. It shows
that intermetallic compound crystallization correlates with bonding duration, as a longer duration is
applied, alumina fragmentation becomes pervasive, resulting in continuous alloy interfaces and robust
bonds. In addition, a substrate temperature (i.e. 175 °C) promotes the fracture of alumina, and simultaneously
contributes to the interfacial temperature, accelerating interdiffusion and facilitating the formation
of intermetallic compounds, therefore increasing bonding strength. The compound formed during
bonding is CuAl2, regardless of the bonding parameters applied.
Ó 2010 Elsevier Ltd. All rights reserved.
materials (Al 660 °C, Au 1063 °C and Cu 1083 °C). In addition,
bonding was successfully performed in liquid nitrogen at 77 K
and without any bubbles being observed, implying that temperature
rise is not a must for bonding [1,17]. Furthermore, a TEM
examination of the bond interface indicated no evidence of melting
. The fretting theory was proposed by Hulst and Lasance 
who argued that interfacial sliding between a wire and a pad cleaning
and heating surface is a key for bonding. However, a measurement
of the movement of the wire during bonding using a laser
interferometer by Wilson  showed that the wire position remained
fixed relative to the substrate during bonding, although
the capillary tool moved with an amplitude of 0.5–2.5 lm, so
bonding can be successful even when there is no interfacial motion.
In addition, the sliding model predicted preferential bonding
at the centre of the interface; however it was reported that bonding
initiated near the periphery [4,20]. Chen  introduced Mindlin’s
micro-slip theory  to explain the interfacial characteristics
of wire bonds. In the proposed model, the central contact region
was termed an elastic or non-slip region, while the outer contact
area was represented as an exhibiting slip, termed a micro-slip.
This fits the commonly observed pattern of the bonds where bonding
predominated at the edge of the contact area rather than at the
centre. All those mechanisms assume that removal of a ubiquitous
native alumina overlayer is essential for successful bonding as it
acts as a barrier to diffusion, and recently, this has been verified
experimentally in our previous work by high resolution transmission
electron microscopy (HRTEM) . It showed that the ultrasonic
vibration under certain pressure and heat partially
fragments the native alumina layer ( 10 nm thick), providing the
114 H. Xu et al. / Microelectronics Reliability 51 (2011) 113–118
pathways for Cu–Al interdiffusion. This promotes formation of the
intermetallic compounds (IMCs) and consequently improves the
bonding strength significantly. On the other hand, the influence
of bonding parameters – ultrasonic power, bonding force, bonding
duration and substrate temperature – on bonding strength were
well documented [8,21–23]. Nonetheless, a full account of the
underlying mechanistic aspects has not been presented, since there
were few reports on interfacial structural changes due to variation
of bonding parameters.
In this paper, the effects of bonding duration and substrate temperature
on the behaviour of the interfacial microstructure (alumina,
IMCs, defects, etc.) was investigated using dual beam
focused ion beam (FIB) and HRTEM. A relationship between those
parameters, interfacial structure and bonding strength is
2. Experimental methods
Thermosonic copper ball bonding was conduced with an ASM
Eagle 60AP ball/wedge automatic bonder. The copper wire
(99.99 wt.%) was 20 lm in diameter with a break strength of
4.3–9.2 gf (1 gf = 9.8 mN) and an elongation of 5–15%. The aluminium
pad is 1 lm thick on SiO2/Si. An electrical flame off
(EFO) process with a 48 mA current, 4500 V gap voltage and
290 ls discharge time produced a free air ball (FAB) at the copper
wire tip. Specifically, a shielding gas (95% N2–5% H2) with
the gas flow rate of 0.6 l/min was utilized to prevent the oxidation
of copper during EFO ball formation. After cooling, the copper
ball was transferred onto the bond pad to form the Cu/Al
bond using a combination of a normal force, transverse ultrasonic
vibration and heat. Three bonding duration settings (levels
BT1, BT2 and BT3) (Table 1) and three substrate temperature settings
(ST1, ST2 and ST3) (Table 2) were selected so that their effects
on the interfacial structure and bonding strength could be
Bonding parameters for three levels of bonding duration a .
studied. To reduce post-thermal effects on interfacial characteristics,
the bonded samples were removed immediately from the
work stage, but inevitably maintained at substrate temperature
Cross-sections of the Cu/Al bonds were prepared by FIB for
scanning electron microscopy (SEM) and transmission electron
microscopy (TEM) analysis. All TEM samples were selected from
the central regions of the interface, an example of which is shown
in Fig. 1. The nanostructure at the interface, including alumina and
IMCs, were investigated by TEM combined with energy dispersive
X-ray spectrometry (EDX). TEM analysis was carried out using a
Bonding parameters Level-BT1 (short duration) Level-BT2 (standard) Level-BT3 (long duration)
Standby power b , DAC 12 (210.0 nm) c
12 (210.0 nm) 12 (210.0 nm)
Contact power, DAC d
10 (175.0 nm) 10 (175.0 nm) 10 (175.0 nm)
Contact force, mN 220 220 220
Contact duration, s 0.001 0.003 0.005
Bonding power, DAC 36 (630.0 nm) 36 (630.0 nm) 36 (630.0 nm)
Bonding force, mN 180 180 180
Bonding duration, s 0.002 0.006 0.010
Substrate temperature, °C 175 175 175
A whole bonding duration consists of two basic stages: (i) contact stage and (ii) bonding stage. During the contact stage, a high bonding force and a low ultrasonic power
are usually employed to cause big plastic deformation of the balls; during the bonding stage, a low bonding force and a high ultrasonic power are used to ensure robust bonds.
Interdiffusion and IMC formation take place during the latter stage, so the bond strength is mainly determined by the bonding stage.
Standby power is ultrasonic power used before the contact stage.
Ultrasonic amplitudes of the capillary tip are listed in brackets.
DAC is an ASM internal energy unit. It is the abbreviation of digital to analog conversion.
Bonding parameters for three levels of substrate temperature.
Fig. 1. Region-specific TEM sample preparation using FIB.
Bonding parameters Level-ST1 (room temperature) Level-ST2 (standard, 175 °C) Level-ST3 (300 °C)
Standby power, DAC 12 (210.0 nm) 12 (210.0 nm) 12 (210.0 nm)
Contact power, DAC 10 (175.0 nm) 10 (175.0 nm) 10 (175.0 nm)
Contact force, mN 220 220 220
Contact duration, s 0.003 0.003 0.003
Bonding power, DAC 36 (630.0 nm) 36 (630.0 nm) 36 (630.0 nm)
Bonding force, mN 180 180 180
Bonding duration, s 0.006 0.006 0.006
Substrate temperature, °C 25 175 300
JEOL 2100F system at 200 kV. A microprobe beam (0.7 nm diameter)
was used for composition analysis with EDX in scanning
(S)TEM mode. Fast Fourier transformation (FFT) of lattice images
calculated using ImageJ 1.42q  was utilized to identify Cu–Al
The shear tests were conducted with a DAGE 4000 micro-tester
at a tool height of 3 lm and a tool movement speed of 4 lm/s. To
avoid the effect of squeezed Al pad on bonding force, the shear
tests were performed to the vertical direction of the ultrasonic
vibration during wire bonding. The load that causes the fracture
of the bonds is termed shear force. The shear strength was obtained
as pressure, i.e. shear force per unit area. The dimension
of the bonds were defined by two parameters – ball diameter D
and ball height H. D =(D A + D B)/2, where D A and D B are the diameters
of the mashed ball along and vertical to the direction of the
ultrasonic vibration, respectively. The ball diameter is usually used
to roughly represent the bonding area. The ball height H is the distance
between the top surface of the bond pad and the edge of the
mashed ball. The values of DA, DB and H were recorded by Olympus
STM6 optical microscopy. 20 bonds were measured at every
3. Results and discussion
3.1. Effect of bonding duration
Shear tests were performed to evaluate the bonding strength
as a function of bonding duration and the results are given in
Table 3. There is a trend of shear strength increases with
increasing bonding duration. A slight increase of ball diameter
D and decrease of ball height H are seen as the bonding duration
In order to understand the underlying mechanism of bonding
duration dependence of bonding strength, the interfacial structure
formed with different bonding duration levels was examined
by electron microscopy. Fig. 2a–c shows the overview of the
interfaces with three levels of bonding duration. There is no significant
difference in the interfacial structure at micro-scale, as
observed by SEM at the magnification level shown in Fig. 2. In
order to characterize the interfacial structure at nano-scale and
verify the difference due to the variation of bonding duration,
TEM analysis was performed.
A typical TEM image of the Cu–Al interface produced with a
short bonding duration (level-BT1) is given in Fig. 3a which shows
that only a few IMC particles are formed and they are approximately
20 nm thick. One location of the IMC particle (region A,
Fig. 3a) with ordered atomic arrays was selected and the lattice image
was collected (Fig. 3b). FFT analysis was consistent with CuAl2
[0 0 1] (Fm-3m, a = 5.9988 Å)  joined with Al (Fm-3m,
a = 4.0496 Å) . In the regions where IMCs are absent, a continuous
and compact layer 5–10 nm thick is situated between the
copper ball and the aluminium pad (Fig. 3c). The STEM–EDX results
Effect of bonding duration on bond dimension, shear force and shear strength.
Fig. 2. SEM images showing the overview of the Cu–Al interfaces with three levels
of bonding duration: (a) level-BT1; (b) level-BT2; (c) level-BT3. *A layer of Pt was
deposited in order to obtain a cleaner cross section.
(Table 4) show that the main constituents of this layer are aluminium
and oxygen, indicating the existence of alumina film which remains
intact after bonding.
As longer bonding duration is applied, more IMCs are formed
along the interface. In particular, a standard value (level-BT2)
results in an almost continuous layer of IMCs (30–40 nm thick)
in regions that were examined (Fig. 4a). Fig. 4b gives a higher magnification
TEM image taken in region A of Fig. 4a, which presents
the morphology of IMC particles. The IMC particles have a conchoidal
interface linked to Al and almost linear interface with Cu, indicating
the growth of those IMCs is dependent on the interdiffusion
of Cu, i.e. Cu diffuse through IMCs to reacts with Al at the IMC/Al
interface. STEM–EDX results (Table 4) show that the IMC is an aluminium-rich
alloy. As a further confirmation, a lattice image
(Fig. 4c) was collect in region A-1 of Fig. 4b and FFT is consistent
with CuAl2 [0 0 1] (Fm-3m, a = 5.9988 Å).
As proposed in our previous work , the initial formation of
IMCs depends on the oxide rupture by ultrasonic vibration at certain
pressures and temperatures. The effect of bonding duration on
the removal of the oxide layer can be described by an equation
developed for a contact surface pair in relative motion :
d ¼ t
where d is the depth of material worn, t is time, P is the mean or
nominal pressure, H is the hardness of the material, k is the
Level-BD1 (short duration) Level-BD2 (standard duration) Level-BD3 (long duration)
Min 37.2 12.7 12.1 – 39.5 11.6 14.1 – 40.6 10.1 15.9 –
Max 39.7 14.2 14.8 – 40.9 12.9 17.4 – 44.8 11.5 20.9 –
Mean 38.4 13.4 13.5 116.6 40.1 12.2 15.5 122.8 42.9 10.9 18.8 130.1
1.08 0.42 0.62 – 0.49 0.45 0.65 – 0.70 0.56 1.06 –
a Standard deviation for 20 measured samples.
H. Xu et al. / Microelectronics Reliability 51 (2011) 113–118 115
116 H. Xu et al. / Microelectronics Reliability 51 (2011) 113–118
Fig. 3. (a) TEM image presenting interfacial morphology of the Cu–Al bond with a
short bonding duration (level-BT1 in Table 1 for detailed bonding parameters); (b)
lattice image and Fourier reconstructed pattern of region A in (a) with CuAl 2 [0 0 1]
linked to the Al pad; (c) details of region B in (a) showing a 5–10 nm thick alumina
layer between the copper ball and the aluminium pad.
STEM–EDX results for regions 1–3 in Fig. 3c and 4–8 in Fig. 4b. The precision of EDX
measurement of O is approximately ±10%, and Al and Cu are approximately ±2%.
Regions O (K at.%) Al (K at.%) Cu (K at.%)
1 6 93 1
2 54 44 2
3 2 8 90
4 6 91 3
5 9 60 31
6 13 58 29
7 7 10 83
8 6 9 85
wear-coefficient constant, and v is the sliding velocity. Thereby, an
increased bonding duration will lead to more sufficient removal of
the oxide layer on the aluminium pad, and therefore more IMCs will
be formed, resulting in a significant increase in the bonding strength.
In addition, a longer interdiffusion results in thicker IMCs in Cu–Al
bonds (from 20 nm for level-BT1 to 30–40 nm for level-BT2), which
may also benefit to the bonding strength. However, the intermetallic
phase remains the same as CuAl2.
3.2. Effect of substrate temperature
A slightly increased bond deformation (larger ball diameter and
smaller ball height) is seen by a higher substrate temperature (Table
5). Moreover, There is an obvious trend of shear strength with
an increase in substrate temperature.
At room temperature (level-ST1), the alumina occupies almost
the interfacial regions (Fig. 5a), as confirmed by a high magnification
TEM image (Fig. 5b) which further shows that the alumina
layer is uniform and compact. The integration of the alumina acts
as a barrier to interdiffusion of Cu and Al, so IMCs is unlikely to
form in those regions. However, if the alumina layer is fragmented,
the formation of IMCs is possible. Only a few IMC particles are
formed during bonding at room temperature (Fig. 5a). Such IMCs
are approximately 20 nm thick, as shown in Fig. 5c, taken from region
B in Fig. 5a. As mentioned earlier, although the bonded samples
were removed immediately after bonding from the work
stage, they were inevitably maintained at the substrate temperature
for 5 s. Wire bonding at room temperature was performed
with the particular aim of eliminating that post annealing. The
presence of IMCs indicates that nucleation and growth of IMCs take
place during bonding, although the quantity of IMCs is small at
room temperature. However, A 175 °C (level-ST2, i.e. standard
bonding parameters) results in an almost continuous IMC layer
in regions that were examined (Fig. 4a). It is inferred that preheating
of substrate promotes the fracture of alumina. Moreover,
a pre-temperature will contribute to the actual Cu–Al interfacial
temperature, accelerating interdiffusion of Cu and Al and facilitating
the formation of IMCs. The formation of IMCs significantly
increases the bonding strength.
According to the equilibrium phase diagram of the Cu–Al system
, at least five intermetallic compounds – CuAl 2(h),
CuAl(g2), Cu4Al3(f2), Cu3Al2(d) and Cu9Al4(c1) – possibly exist.
However, only CuAl 2 is formed during bonding. Using the model
of Pretorius et al. [29,30], with the effective concentration of
17 at.% Cu 83 at.% Al, the effective heats of formation for CuAl 2,
CuAl and Cu9Al4 are estimated to be 6.1 kJ/mol, 5.1 kJ/mol and
4.1 kJ/mol, respectively; therefore, CuAl 2 is the favoured phase
to be formed. This is consistent with the results in this study that
CuAl 2 nucleates during bonding, which is also in agreement with
a previous TEM study by Drozdov et al. . In addition, from
the crystallographic point of view, the more atoms there are in a
unit cell, the more difficult and less energetically favourable it is
to crystallize. CuAl 2 (tetragonal, I4/mcm) [31,32] has 12 atoms
Fig. 4. (a) TEM image presenting interfacial morphology of the Cu–Al bond with a
standard bonding parameters (level-BT2 in Table 1 for detailed bonding parameters);
(b) details of regions A in (a) showing the morphology of IMC particles; (c) lattice
image and Fourier reconstructed pattern of region A-1 in (b) with CuAl2 [0 0 1].
H. Xu et al. / Microelectronics Reliability 51 (2011) 113–118 117
Fig. 5. (a) TEM images showing an overview of the Cu–Al interface formed at room
temperature; (b) details of region A in (a) presenting a uniform layer of alumina
between the copper ball and the aluminium pad; (c) details of region B in (a)
presenting approximately 20-nm-thick IMC particles.
per unit cell and a short range order, and is more likely to be
formed than CuAl (monoclinic, C12/m1, 20 atoms per unit cell)
 and Cu9Al4 (cubic, P4–3m, 52 atoms per unit cell) . Thus,
it is reasonable to believe that CuAl 2 nucleates first during wire
bonding. Such initial IMC layer will grow if the bonds undergo
post-thermal annealing, and Cu 9Al 4 and CuAl may emerge, as has
been reported that Cu9Al4 and/or CuAl were also formed after
annealing depending on annealing conditions by electron diffraction
 and Micro X-ray diffraction analysis . In thin-film
studies (where Al and Cu films were deposited one by one without
breaking the vacuum) X-ray diffraction and Rutherford backscattering
spectrometry found that CuAl 2 was formed initially
[37,38], while elsewhere CuAl2 and Cu9Al4 [39–41] reportedly
118 H. Xu et al. / Microelectronics Reliability 51 (2011) 113–118
Effect of substrate temperature on bond dimension, shear force and shear strength.
The effects of bonding duration and substrate temperature on
interfacial microstructure and bonding strength were investigated
to establish a bonding process – microstructure – property relationship.
The obtained results show that:
(1) IMC crystallization correlates with bonding duration, as a
longer duration is applied, alumina fragmentation becomes
pervasive resulting in continuous alloy interfaces and therefore
(2) The interfacial structure and bonding strength are also
dependent on substrate temperature. Only a few IMCs are
formed during bonding at room temperature, while elsewhere
there are uniform layers of alumina. Pre-heating of
substrate promotes the fracture of alumina, and simultaneously
contributes to the actual interfacial temperature,
accelerating interdiffusion and facilitating the formation of
IMCs, therefore increasing bonding strength.
(3) The compound formed during bonding is CuAl2, regardless of
the bonding parameters applied. The Cu–Al bonds is voidfree
in the as-bonded state.
This research was funded as a PMI2 Project (Grant No. RC 41)
through the UK Department for Innovation, Universities and Skills
(DIUS) for the benefit of the Singapore and the UK Higher Education
Level-ST1 (room temperature) Level-ST2 (175 °C) Level-ST3 (300 °C)
 Joshi KC. The formation of ultrasonic bonds between metals. Weld J
 Mayer M, Paul O, Bolliger D, Baltes H. Integrated temperature microsensors for
characterization and optimization of thermosonic ball bonding process. IEEE
Trans Compon Pack Technol 2000;23:393–8.
 Ho JR, Chen CC, Wang CH. Thin film thermal sensor for real time measurement
of contact temperature during ultrasonic wire bonding process. Sensors
Actuators A: Phys 2004;111:188–95.
 Harman GG, Albers J. The ultrasonic welding mechanism as applied to
aluminum-and gold-wire bonding in microelectronics. IEEE Trans Parts
Hybrids Pack 1977;13:406–12.
 Lum I, Jung JP, Zhou Y. Bonding mechanism in ultrasonic gold ball bonds on
copper substrate. Metall Mater Trans A 2005;36:1279–86.
 Lum I, Mayer M, Zhou Y. Footprint study of ultrasonic wedge-bonding with
aluminum wire on copper substrate. J Electron Mater 2006;35:433–42.
 Zhou Y, Li X, Noolu NJ. A footprint study of bond initiation in gold wire crescent
bonding. IEEE Trans Compon Pack Technol 2005;28:810–6.
 Qi J, Hung NC, Li M, Liu D. Effects of process parameters on bondability in
ultrasonic ball bonding. Scripta Mater 2006;54:293–7.
 Xu H, Liu C, Silberschmidt VV, Chen Z, Wei J. The role of bonding duration in
wire bond formation: a study of footprints of thermosonic gold wire on
aluminium pad. Microelectron Int 2010;27:11–6.
 Xu H, Liu C, Silberschmidt VV, Pramana SS, White TJ, Chen Z. A re-examination
of the mechanism of thermosonic copper ball bonding on aluminium
metallization pads. Scripta Mater 2009;61:165–8.
Min 37.4 11.7 7.2 – 39.5 11.6 14.1 – 39.1 10.7 19.1 –
Max 40.9 13.5 9.5 – 40.9 12.9 17.4 – 44.5 12.1 23.9 –
Mean 39.1 12.6 8.3 69.2 40.1 12.2 15.5 122.8 42.8 11.5 21.2 147.4
0.81 0.53 0.80 – 0.49 0.45 0.65 – 0.89 0.45 1.32 –
a Standard deviation for 20 measured samples.
 Drozdov M, Gur G, Atzmon Z, Kaplan W. Detailed investigation of ultrasonic
Al–Cu wire-bonds: I. Intermetallic formation in the as-bonded state. J Mater
 Tian YH, Wang CQ, Zhou Y. Investigation of ultrasonic copper wire wedge
bonding on Au/Ni plated Cu substrates at ambient temperature. J Mater
Process Technol 2008;208:179–86.
 Winchell VH, Berg HM. Enhancing ultrasonic bond development. IEEE Trans
Compon Hybrids Manuf Technol 1978;1:211–9.
 Hulst AP, Lasance C. Ultrasonic bonding of insulated wire. Weld J
 Chen GKC. The role of micro-slip in ultrasonic bonding of microelectronic
dimensions. Int Hybrid Microelectron Symp 1972;5A:111–9.
 Mindlin RD. Compliance of elastic bodies in contact. J Appl Mech
 Harman GG, Leedy KO. An experimental model of the microelectronic
ultrasonic wire bonding mechanism. In: Proc. 10th annual proc. reliability
physics, Las Vegas, USA; 1972. p. 49–56.
 Krzanowski JE. A transmission electron microscopy study of ultrasonic wire
bonding. IEEE Trans Compon Hybrids Manuf Technol 1990;13:176–81.
 Wilson AD. Holographic interferometry applied to motion studies of ultrasonic
bonders. IEEE Trans Sonics Ultrasonics 1971;19:453–61.
 Johnson KL. One hundred years of Hertz contact. Proc Inst Mech Eng
 Lum I, Huang H, Chang BH, Mayer M, Du D, Zhou Y. Effects of superimposed
ultrasound on deformation of gold. J Appl Phys 2009;105:024905-5.
 Xu H, Liu C, Silberschmidt VV, Wang H. Effects of process parameters on
bondability in thermosonic copper ball bonding. In: 58th Electronic
components and technology conference; 2008. p. 1424–30.
 Ding Y, Kim JK, Tong P. Effects of bonding force on contact pressure and
frictional energy in wire bonding. Microelectron Reliab 2006;46:1101–12.
 Rasband W. ImageJ Version 1.42q. Bethesda, Maryland, USA: National
Institutes of Health; 2009. .
 Buchler H, Range KJ. Hochdruck–Hochtemperatursynthese und kristallstruktur
von Al 11 Au 6 und AlAu. J Less Common Metals 1990;160:143–52.
 Downs RT, Hall-Wallace M. The American mineralogist crystal structure
database. Am Mineral 2003;88:247.
 Peterson MB, Winer WO. Wear control handbook. New York: ASME; 1980.
 Murray JL. The aluminum–copper system. Int Metals Rev 1985;30:211–33.
 Pretorius R, Theron CC, Vantomme AC, Mayer JC. Compound phase formation
in thin film structures. Crit Rev Solid State Mater Sci 1999;24:1–62.
 Pretorius R, Vredenberg AM, Saris FW, de Reus R. Prediction of phase formation
sequence and phase stability in binary metal–aluminum thin-film systems
using the effective heat of formation rule. J Appl Phys 1991;70:3636–46.
 Meetsma A, de Boer JL, van Smaalen S. Refinement of the crystal structure of
tetragonal Al 2Cu. J Solid State Chem 1989;83:370–2.
 Owen EA, Preston GD. X-ray analysis of solid solutions. Proc Phys Soc
 El-Boragy M, Szepan R, Schubert K. Crystal structure of Cu3Al2 + (h) and CuAl
(r). J Less Common Metals 1972;29:133–40.
 Arnberg L, Westman S. Refinement and test of twinning of the gamma-Cu 9Al 4
structure. Acta Crystallogr A 1978;34:399–404.
 Drozdov M, Gur G, Atzmon Z, Kaplan W. Detailed investigation of ultrasonic
Al–Cu wire-bonds: II. Microstructural evolution during annealing. J Mater Sci
 Kim HJ, Lee JY, Paik KW, Koh KW, Won JH, Choe SY, et al. Effects of Cu/Al
intermetallic compound (IMC) on copper wire and aluminum pad bondability.
IEEE Trans Compon Pack Technol 2003;26:367–74.
 Gershinskii AE, Fomin BI, Cherepov EI, Edelman FL. Investigation of diffusion in
the Cu–Al thin film system. Thin Solid Films 1977;42:269–75.
 Tamou Y, Li J, Russell SW, Mayer JW. Thermal and ion beam induced thin film
reactions in Cu–Al bilayers. Nucl Instrum Methods Phys Res Section B
 Campisano SU, Costanzo E, Scaccianoce F, Cristofolini R. Growth kinetics of hphase
in Al–Cu thin-film bilayers. Thin Solid Films 1978;52:97–101.
 Rajan K, Wallach ER. A transmission electron microscopy study of intermetallic
formation in aluminium–copper thin-film couples. J Cryst Growth
 Hamm RA, Vandenberg JM. A study of the initial growth kinetics of the
copper–aluminum thin-film interface reaction by in situ X-ray diffraction and
Rutherford backscattering analysis. J Appl Phys 1984;56:293–9.